graphic hand-painted blue-and-white porcelain manufacturing process
1. Rub the mud.
The purpose of kneading mud is to empty the air bubbles in the mud and make it more compact.In the absence of this process, it is easy to appear in the body contains bubbles, the body dry-fired deformation is easy to rupture.
2. Making Blank
Jingdezhen traditional round tool is made of the body according to the final type, which can be used for later printing.
3. Print blank
Good rough, after a certain time of natural shade dry (must be in a certain humidity and temperature conditions natural shade dry, not sun. The billet body that does billet form, must be on billet board slant, cannot be placed upright, upright place, the billet that can produce bottom is cracked), can enter printing billet process.The purpose of the printing blank is to make the hand-formed circular ware uniform after firing.After the billet is naturally dry by hand, the semi-dry billet is placed on the earth grinding tool and clapped by hand.
The sharp billet is the finishing of the printed billet to make it smooth and round further.
5. Dang Li Glaze
Round making, if there is no decoration in the device, you need to put on the inner glaze first.The glaze on the outside of the object is the second dip in the later period.Glaze is a vitreous thin layer attached to the surface of ceramic body, which has similar physical and chemical properties to glass.Glazes are usually made of quartz, feldspar, clay, etc.The methods of glazing include spraying, blowing, soaking, pouring and swamping.The inner glaze (the inside of the object) and the bottom glaze (the base of the object) we adopt the traditional roll glaze method, we use the outer glaze method.
The billet of good billet of inside glaze, can enter drawing billet process.
The green flower material used for drawing billet needs to be ground for a long time in advance, and the formula is indescribable in every studio.
To hook up:
The charm of blue-and-white porcelain is like the position of freehand painting in Chinese traditional painting, and the beauty of blue-and-white not only in fine painting, but also in the beautiful and delicate layers of traditional Chinese painting and painting. And it all comes from mixing water.
7. Exterior glazes
Draws the finished porcelain billet, needs to carry on the second glazing process.At this point, the bottom of the cup has not yet formed.Immersion method needs to master the body, glaze and porcelain expected to have a comprehensive understanding and grasp.The length of time the porcelain billet is immersed in the glaze water directly affects the quality of the porcelain after firing.
After glaze is applied outside porcelain billet, after glaze surface is naturally dry, can enter the process of digging bottom foot.Because what we make is glaze foot thing, when excavating base foot, need to leave the billet of the outermost circle of base foot, and must keep the same of outer circle, this needs very strong control ability and work base.
9. Write the bottom and apply the bottom glaze.
10. Glazed feet
Glazed feet, the initial state is in the ceramic wheel hand-made small round mud cake.After drying again in the ceramic wheel spin out the corresponding shape, and each cup one-to-one.
With glaze foot branch burning technology, only in the official kiln firing court porcelain, the use of glazed foot branch burning porcelain pottery foot is full of glaze, that is, beautiful, smooth and not to scratch the surface of furniture, but because of the complexity and difficulty of this process, Modern ceramic industry only uses this process to make expensive high-grade porcelain.
11. Full Kiln, Burning Kiln
The porcelain billet to be burned is distributed reasonably in the kiln body, which is called full kiln.When the kiln is full, it needs to be arranged according to the structure of the kiln body and the size of all the billet body to be burned properly, and set aside a reasonable flue of fire, otherwise it will affect the atmosphere of the kiln body when the kiln is fired, leading to the failure of the firing.
Jingdezhen traditional blue-and-white porcelain used reduction firing, we fired the temperature of 1330 ° C, burning time of about 10 hours.
12. Opening a Kiln
After 12-18 hours of natural cooling, in the kiln body temperature drops to normal temperature, can open the kiln.This is the most exciting moment in the entire production process.
Finally, we need to test the porcelain and polish the bottom of the kiln.
Each piece of hand-made ceramic products from kneading mud to burning finished, experienced dozens of process key technical points, each from a series of artists over the years accumulated skills, have experienced a stroke of careful drawing.Even a similar content is also each with its own unique life, after reading the above content, you will also think that such a handmade ceramic products is only a cheap commodity?
Hand-handed inheritance for thousands of years, continued to this day, the decline of a lot of skills, that superb, fine level of technology, is now unattainable.After counting the years, you can enjoy the pleasure of hand-made.